Failure Mode Predictions in the Compressive Response of Laminated Composites


 Dwight Copeland
 1 years ago
 Views:
Transcription
1 Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA Failure Mode Predictions in the Compressive Response of Laminated Composites Pavana Prabhakar and Anthony M Waas Of interest in this paper are failure mode interactions when laminated fiber reinforced composites are subjected to compressive loading. Delamination, fiber kinkbanding and their interactions are seen to dominate the failure response. This interaction is captured through a computational model that includes interface elements to capture delamination, and, geometric and material nonlinearity to capture kink banding. A 2D crosssection analysis is used to guide the choice of interfaces that require cohesive elements, thus reducing computational complexity. Two different stacking sequences are investigated, and their compressive strength and failure modes are compared, between prediction and experiments. I. Introduction Fiber kink banding has been identified as a compressive strength limiting mechanism in aligned fiber reinforced composite laminates that are finding increasing use in lightweight aerostructures (Schultheisz and Waas, 1 Waas and Schultheisz 2 ). While early studies determined that the compressive strength can be determined by a knowledge of the shear nonlinearity in the stressstrain response of a lamina in tandem with a knowledge of initial fiber misalignment, 3, 4 it was later determined through a combination of experiments and numerical modeling that the kink band formation is an evolutionary process, leading to deformation localization. The mechanism is governed by local stress state (including stress multiaxiality), details of the material constitutive model and the fiber misalignment angles as explained in papers by Sun and Jun, 5 Kyriakides et al., 6 Lee and Waas, 7 Vogler et al., 8 Yerramalli and Waas, 9 Yerramalli and Waas, 10 Basu et al., 11 Pimenta et al., 12, 13 Feld et al. 14 As loading proceeds, regions of fiber misalignment in the composite undergo deformation due to combined compression and shear loading. This region is surrounded by other material whose deformation characteristics, in general, are different. The progressively increasing local fiber misalignment coupled with a softening shear nonlinearity, perpetuates a local limitload type instability that initiates a rapid formation of a kink band. During this formation, the external tractions required to support the structure, in general, decrease, indicating an instability. The regions within the band undergo large straining while material outside the band, relax and unload. Consequently, the mechanics of this process is related to the local microstructural details, geometry and volumes of material that are occupied by the band and that which are outside the band. Lee and Waas, 7 Lee et al., 15 Vogler et al. 8 and Pimenta et al., 12, 13 have shown that kinkband formation can also involve delamination (splitting) in combination or in isolation of the band formation. Lee and Waas 7 studied the effect of fiber volume fraction on the compression failure mode, while Yerramalli and Waas 9 studied the effect of fiber type and load multiaxiality on failure. The formation of kink banding as an energy release mechanism in limiting the compressive strength of laminates with cutouts has previously been addressed by Waas et al., 16 Ahn and Waas, 17, 18 and Berbinau et al., 19 while the influence of fiber waviness on compression failure of unidirectional laminates has been studied by Wisnom. 20 Micromechanical models to predict compressive strength using varying degrees of simplification have been proposed by Naik and Kumar, 21 and, Xu and Reifsnider. 22 While kink banding is governed by the inelastic response of the matrix material in a misaligned fiber composite, delamination is governed by the fracture properties of the matrix and/or fiber matrix interface,. 23 Graduate Student, Department of Aerospace Engineering, 1320 Beal Avenue, Ann Arbor, MI AIAA Student Member. Felix Pawlowski Professor of Aerospace Engineering, Department of Aerospace Engineering, 1320 Beal Avenue, Ann Arbor, MI Fellow, AIAA. 1 of 15 Copyright 2013 by Pavana Prabhakar. Published by the, Inc., with permission.
2 In this paper, multidirectional carbon fiber reinforced polymer (CFRP) matrix laminates are considered. The main goal of this paper is to develop a procedure to predict compressive strength and failure modes in multidirectional laminates. In this regard, a semihomogenized laminate model is constructed, where micromechanics is maintained in the 0 degree fibers and the offaxis layers are homogenized. Further, to predict the compressive strength and failure modes, cohesive elements are added at chosen interfaces of the model to incorporate the ability to delaminate. These interfaces are determined a priori by a simplified 2D analysis of the laminate. The compressive strength and failure modes are predicted for two laminates with different stacking sequence, and compared against experimental observations and test data. Two types of laminates with different stacking sequence are studied here. The first type of laminate, namely, Type A laminates, have a stacking sequence of [ 45/ + 45/90/0]s, [ 45 2 / /90 2 /0 2 ]s and [ 45 4 / /90 4 /0 4 ]s with totals of 8, 16 and 32 layers, respectively. The second laminate is referred to as Type B laminate, with a stacking sequence of [( 45/+45/90/0) 6 ]s, with 48 layers. It should be noted that the zero degree layers are grouped together along the centerline in Type A laminate, whereas they are distributed in the Type B laminate. Upscaled homogenized laminate models are constructed for both types of laminates using the upscaled semihomogenized modeling method explained in Prabhakar and Waas. 24 In these models, each 0 degree lamina has hexagonally packed fibers maintaining the micromechanics, and the offaxis layers are homogenized using a deformation theory implementation of Hill s anisotropic plasticity theory. Interface elements formulated using the discrete cohesive zone method (DCZM) (Gustafson and Waas 25 ), are added at the critical interfaces which are determined apriori as the delamination prone interfaces in the laminate, via a simplified 2D analysis of the laminate. Finally, the laminate model is subjected to compression in the axial direction, using displacement control, to predict the compressive strength and failure modes. II. A. Type of Laminates Investigated Experimental Observations The two types of laminates investigated are shown in Fig. 1(a) and Fig. 1(c). Different layers are seen in the figures through contrasting colors in the images. The Type A laminate shown in Fig. 1(a) contains 16 layers, and the Type B laminate in Fig. 1(c) contains 48 layers. Both laminates are symmetric about the centerline. B. Compression Test Fixture and Specimens Compression tests were conducted on Type A and Type B laminates to understand the mechanisms of failure that are unique to the different type of laminates. The influence of two important types of failure mechanisms, namely delamination and kinking, and their interaction on the compression strength is the main focus. In the following sections, details about the experimental setup, stacking sequences (also referred to as layups) of different specimens and results of the compression experiments are presented. The Wyoming Combined Loading Compression (WCLC) test fixture was used to carry out the compressive response studies in association with a MTS loading frame. Specimens in the form of strips of laminates with nominal dimensions of 12.7 mm x mm x t mm, where, t is variable, are sandwiched between the large metal blocks of the fixture, and the ends of the fixture are compressed between the flat loading platens of a MTS testing frame. The blocks act as antibuckling guides during loading, supporting a large portion of the specimen length, and providing a length of 6.35 mm as the gage length. This results in the measured compressive strength to be as close as possible to the actual compressive strength of the material, with minimal tendency towards flexural buckling. Specimens of three layups of Type A laminates, with varying thickness, and Type B laminates were tested under compression. The Type A specimens were also used to study the effects of scaling, by grouping families of lamina, on the compressive strength of the laminates. As indicated in Table 1, the thicknesses of the layups are scaled up by stacking multiple layers of the same orientation. All the laminates shown in Table 1 have the same inplane extensional stiffnesses. All the specimens are of nominal size 12.7 mm x mm which results in a nominal gage length of 6.35 mm when placed in the WCLC fixture. Fig. 1(b) displays the image of a failed Type A 16ply laminate. It is observed that the failed specimen shows extensive delamination occurring at the interface of the laminae, and kinking in the 0 degree ply. Fig. 1(d) shows a failed Type B specimen. We observe kink band formation in 0 layers, and small delaminated regions around the kink band are observed. There is no extensive delamination observed in Type B laminates 2 of 15
3 (a) (b) (c) (d) Figure 1. (a) Pristine TypeA laminate; (b) Failed TypeA laminate; (c) Pristine TypeB laminate; (d) Failed TypeB laminate Table 1. Types of laminates Type of Laminates L(mm) W(mm) t(mm) Type A (8 plies): [ 45/ + 45/90/0]s Type A (16 plies): [ 452 / /902 /02 ]s Type A (32 plies): [ 454 / /904 /04 ]s Type B (48 plies): [( 45/ + 45/90/0)6 ]s as in the case of Type A laminates. C. Compressive Strength Measurements The compressive response studies are carried out at an external displacement control loading rate of in/sec in a MTS hydraulic test frame. The macroscopic stress is calculated as the total load obtained from a load cell that is placed inline with the specimen, divided by the initial undeformed cross sectional area of the specimen. The macroscopic strain is determined using strain gages on either faces of the specimens. The global stressstrain responses of Type A laminates are shown in Fig. 2. The initial stiffness of the laminates is 48.5 ± 2 GPa, and the compressive strengths are in the range of 590 ± 30 MPa. The results imply that the scaling of lamina thickness in the laminate has no significant influence on either the initial stiffness or the strength of the Type A laminates. The Type B laminates displayed a similar trend with an initial stiffness of 49.3 ± 0.5 GPa, and the compressive strengths are in the range of 615 ± 20 MPa. 3 of 15
4 Stress (MPa) Ply:Test Ply:Test 2 16 Ply:Test Ply:Test 2 32 Ply:Test 1 32 Ply:Test Strain Figure 2. Global stressstrain response of the Type A laminates determined experimentally D. Strain Analysis of Laminates Using Digital Image Correlation (DIC) The digital image correlation (DIC) method was used to analyze the strain distribution on the side face of the laminates. ARAMIS, a commercially available software package, is used to perform the DIC analysis. ARAMIS is a noncontact and material independent displacement measuring system that gives displacements, strains and velocities as a function of time. 26 The side surface of the specimen (through the thickness), which is to be imaged, has a speckle pattern with random black dots over a white background, created using an airbrush. The side surface that is imaged is the surface with a normal in the y  direction. A series of images are taken during the experiment, and these images are analyzed using ARAMIS to calculate the displacement and strain fields. The DIC images of the side surface of a typical 16ply Type A specimen are shown in Fig. 3(a) and Fig. 3(b). The specimen is loaded in the global xdirection. Fig. 3(a) and Fig. 3(b) display the strain distribution on the side face of the specimen along the global zdirection corresponding to a point prior to peak load and at the peak load of the loaded specimen. It can be observed that the distribution is banded along the thickness. This is due to the different layers present in the specimens. We also observe that, as the loading is increased, the positive strain between the layers +45 and 45 increases rapidly, and subsequently, the specimen delaminates at that interface as clearly shown in Fig. 3(b). To corroborate the above statement, the shear strain distributions ɛ xz along a line on the side face are also plotted. It is clear from Fig. 3(c) that as the load is increased, the shear strain (ɛ xz ) attain maximum values at the interface between +45 and 45 layers. Upon further loading, the transverse and shear strains tend to very large values as the specimen delaminates at the interface on the right (refer to Fig. 3(d)). In summary, the specimens appear to initiate failure by delamination followed by kink band occurring in the postpeak regime. Similarly, the DIC analysis of the Type B 48ply laminate is carried out. The DIC images of the side face of a Type B specimen are shown in Fig. 4(a) and Fig. 4(b). Fig. 4(a) and Fig. 4(b) display the strain distribution on the side face along the global zdirection. Here, distinct strain bands representing each layer in the laminate do not exist, as opposed to Type A laminates. This maybe due to a lack of a sufficiently fine speckle pattern on the side face, and also perhaps the inability of ARAMIS to capture changes between each thin lamina with different fiber orientation in the 48  ply laminate. This is in contrast to Type A laminates where relatively thick clustered layers with the same fiber orientation exist. The strain distributions ɛ xz along a line on the side face are also plotted. We also observe that as the loading is increased, the average strain level along the side face increases, but ARAMIS measurement is unable to capture the behavior of different layers individually. Upon further loading, the shear strain attains large value at the center of the specimen as seen in Fig. 4(d), but with order to magnitude smaller than that in Type A laminate. In summary, assertive conclusions cannot be made based on purely the DIC analysis of Type B specimens regarding the role of interfaces in the failure of these specimens. Since the stacking sequence leads to a rapidly alternating set of 4 of 15
5 (a) (c) (b) Figure 3. Transverse strain distribution on the side surface for TypeA 16ply laminate at (a) point prior to peak load (b) peak load; Shear strain distribution across the side surface for TypeA 16ply laminate at (c) point prior to peak load (d) peak load (a) (d) (c) (b) (d) Figure 4. Transverse strain distribution on the side surface for TypeB 48ply laminate at (a) point prior to peak load (b) peak load; Shear strain distribution across the side surface for TypeB 48ply laminate at (c) point prior to peak load (d) peak load layers, each of relatively small thickness, the field of view used to take images for DIC and the image size does not lead to a sufficiently adequate resolution of the strain field present in these laminates. 5 of 15
6 III. Computational Modeling Upscaled models of homogenized laminates are constructed for two different layups, with stacking of [( 45 2 /+45 2 /90 2 /0 2 )] s (Type A) and [( 45/+45/90/0) 2 ] s (Type B) as explained in Prabhakar and Waas, 24 where the 0 degree layers have a hexagonal packed fibers maintaining the micromechanics, and the offaxis layers are homogenized using Hill s anisotropic plasticity along with deformation theory of plasticity. Interface discrete cohesive zone method (DCZM) elements are added at critical interfaces which are determined a priori. This is determined using a simplified 2D analysis of the laminate which is explained in the following sections. Finally, each laminate model is compressed in the global ydirection to predict the compressive strength and failure modes. A. Upscaled Laminate Model The upscaled homogenized models consist of 16layers of laminae (see Fig. 5 and Fig. 6), where the offaxis layers i.e ,45 0,90 0 layers, are homogenized using the technique mentioned in Prabhakar and Waas. 24 Here, the red, cream and blue regions are the homogenized 45, +45 and 90 degree laminae. Micromechanics is maintained in the 0 0 layers, as they are the load bearing layers and are responsible for kink band formation in multidirectional laminates. Therefore, the regions in green are the 0 degree fibers, and regions in grey are the matrix in 0 degree lamina. Figure layered upscaled model of Type A laminate with homogenized offaxis laminae The homogenized elastic lamina properties of the offaxis laminae corresponding to a fiber volume fraction of 0.49 are given in Table 2 and Fig. 7. Other material properties are given in Table 3. The constants R ij required to implement Hill s anisotropic plasticity model are tabulated in Table 4 (note that R 11 is chosen to be an arbitrarily high value since the 1direction of the lamina is assumed to be elastic throughout). These properties are applied to offaxis laminae in their rotated coordinates accounting for their ply orientations. Table 2. Fiber Properties E 11 (GPa) E 22 (GPa) E 33 (GPa) G 12 (GPa) G 13 (GPa) G 23 (GPa) ν 12 ν 13 ν A schematic of the two models shown in Fig. 8 is further used to describe the boundary conditions and loading on the model. The edge AE of the model is prevented from motion in the zdirection, and the corner E is fixed against moving in the global x, y and zdirections. The face BFGC is subjected to compression along the negative xdirection in a displacement control manner. The faces ABCD and EFGH are held flat 6 of 15
7 Figure layered upscaled model of Type B laminate with homogenized offaxis laminae Equivalent stress (MPa) E s Equivalent strain Figure 7. Equivalent stressstrain curve for the insitu matrix Table 3. Elastic Homogenized Lamina Properties E 11 (GPa) E 22 (GPa) E 33 (GPa) G 12 (GPa) G 13 (GPa) G 23 (GPa) ν 12 ν 13 ν Table 4. Values of R ij for calculating Hill s potential constants R 11 R 22 R 33 R 12 R 13 R but are allowed to expand or contract in the ydirection. Also, the faces ABCD and EFGH deform exactly the same way in x and zdirections. This enables the use of one representative unit cell in the ydirection, along with preserving a constant initial stiffness of the laminate, regardless of the width of the model. 7 of 15
8 Figure 8. A schematic of the laminate model to describe boundary conditions and loading The Riks method option available in ABAQUS v6.10, which is an arclength solution scheme, is adopted to conduct the compressive response analysis. As shown in previous studies, 27 this method captures unstable equilibrium paths (path in the load vs. loaded edge displacement graph that show snapback response) that can occur at limit points, as will be discussed later. The model is meshed with 3D hexahedral elements (C3D8 in ABAQUS v6.10). The macroscopic stress is defined as the total resultant xdirection reaction force on the face BFGC divided by the product of the width BF and thickness BC, while the macroscopic strain is defined as the total contraction (change in length between the faces BFGC and AEHD) divided by the initial length AB. B. 2D reduction formulation to determine a priori interfaces susceptible to delamination in a laminate After developing the upscaled laminate model, the interface most susceptible to delamination needs to be determined in order to add interface elements along that interface. Methods to carry out free edge effects, and to obtain the stresses along the interface of laminates have been formulated and presented in a series of papers by Pipes and Pagano, 28 Pagano et al., 29 Pagano and Pipes, 30 and more recently by Martin et al. 31 A generalized 2D plane strain formulation using the FEM framework presented in Martin et al., 31 but using 3D elements is implemented here, and solved using the FE ABAQUS code. A brief overview of the formulation of the generalized 2D framework is explained in the following section. 1. Mathematical Formulation Based on the formulation given in, 28 and, 31 a laminate of length 2L, width of 2b and lamina thickness equal to h is considered. The geometry of the laminate along with its boundaries is shown in Fig. 9(a). The layers in the laminate are in the x 1 x 2 plane. A compressive load is applied at the edges Σ +L and Σ L along the x 1 direction. Edges Σ 0 and Σ 2b are the free edges in the x 2 direction. A crosssection of the laminate at AA is shown in Fig. 9(b) that has N layers through the thickness. The p th interface between the laminae is represented by Γ p. At a region considerably far from the loading edges, the stress components are assumed to be independent of x 1. That is, the axial strain ɛ 11 is assumed to be uniform along the x 1 direction within the laminate. This behavior was reported in 32 through Moire fringe patterns on the surfaces in the x 1 x 2 plane of different laminates. A region considerably far from the loading surfaces is considered such that the stress components are assumed to be independent of x 1. Then, the displacement field is given as, U 1 (x 1, x 2, x 3 ) = Ũ1(x 2, x 3 ) + ɛ 11 x 1 U 2 (x 1, x 2, x 3 ) = Ũ2(x 2, x 3 ) U 3 (x 1, x 2, x 3 ) = Ũ3(x 2, x 3 ) (1) Here, ɛ 11 is the applied uniform axial strain in the laminate in the x 1 direction. The constitutive law for each linear elastic lamina (3D), in the tensorial form is, σ ij = a ijkl ɛ kl, where, i,j=1,2,3 within the laminate. 8 of 15
9 Here, a ijkl, is the fourth order linear elasticity tensor for a general anisotropic material. At the interface, we must ensure displacement and traction continuity, which are given by, Displacement Continuity : [U i ] = 0 Traction Continuity : [σ ij n j ] = 0 on the interface Γ p (2) At the traction free edges and the loading, we have, σ ij n j = 0 i = 1, 2, 3on Σ 0 and Σ 2b σ ij n j = F i on Σ +L (3) σ ij n j = F i on Σ L Weak form: Let V be a weighting field for the equilibrium equations, given by, V = average of the equilibrium equations are, Ω V 1 (x 2, x 3 ) V 2 (x 2, x 3 ) V 3 (x 2, x 3 ). The weighted σ ij V i x j = 0 (4) Since V = f(x 2, x 3 ) Vi x 1 = 0, which implies the weighting field is independent of x 1. Substituting the constitutive relation for σ ij into the above equation, we have, S Ũk V i a iαkh dx 2 dx 3 = ɛ 11 a iα11 V i n α ds (5) x h x α S where, s represents a coordinate that denotes the boundary S, starting at the origin of the x 2 x 3 axes for the region S, and traversing in an anticlockwise direction. Therefore, s is either x 2 or x 3 depending on the portion of the boundary being traversed. The above equation is modified to account for layers with different orientation in a multidirectional laminate as given below, N p=1 a p Ũ p k iαkh S p V p N i dx 2 dx 3 = ɛ 11 x h x α p=1 S p a p iα11 V p i np αds (6) Equation 7 is a generalized 2D formulation which has displacement fields along the x 1,x 2 and x 3 directions, but in a 2D (x 2 x 3 plane) domain. The input to the above formulation is the 4th order elasticity tensor of each layer of the laminate for a linear elastic material and the applied external strain. The equivalent loads calculated for a laminate are applied to the 2D generalized representation of the laminate in the FEM model given in the next section. 2. Implementation of the Generalized 2D Formulation The 2D generalized plane strain formulation presented above can be implemented in several ways using the finite element method. The method used here is to modify a thin slice of a 3D model to behave like a generalized 2D model. A 3D model of a laminate (shown in Fig. 9(a)) with a small thickness in the xdirection is considered as shown in Fig. 2. The model is restricted from any expansion in the xdirection using multipoint constraints. This satisfies the requirement that the displacement fields are independent of the xdirection. This gives us the left hand side of equation (7) (refer to Martin et al. 31 ). N p=1 a p Ũ p k iαkh S p V p N i dx 2 dx 3 = ɛ 11 x h x α p=1 S p a p iα11 V p i np αds (7) The external loads are applied to the model on the edges in the yz plane (refer to Fig. 9(b)) and the interfaces between the layers. 9 of 15
10 (a) (b) Figure 9. (a) 3D laminate; (b) Crosssection of the 3D laminate Figure D slice of a laminate 10 of 15
11 3. Determination of Delamination Prone Interfaces in Laminates The above formulation is implemented for an 8ply laminate with a stacking of [45/+45/90/0]s (half of the laminate is used as shown in Fig. 11(a)) to determine the weak interfaces. Fig. 11(b) shows the strains ɛ 33,ɛ 13 and ɛ 23 along the 45/+45 (Interface 1), +45/90 (Interface 2) and 90/0 (Interface 3) interfaces. It is observed in Fig. 11(b) that ɛ 13 is very high at Interface 1 as compared to the strains at the other Interfaces. Therefore, Interface 1 is considered to be the interface that is most susceptible to delaminate. This information will be used in constructing the computational model of the laminate, i.e. the cohesive elements will be added along Interface 1 to allow for delamination at 45/+45 interfaces. Strain (a) Interface 1 :ε 33 Interface 1 :ε 13 Interface 1 :ε 23 Interface 2 :ε 33 Interface 2 :ε 13 Interface 2 :ε 23 Interface 3 :ε 33 Interface 3 :ε 13 Interface 3 :ε Normalized length along cross section (b) Figure 11. (a) Symmetric model representing an 8ply laminate with a stacking of [ 45/ + 45/90/0] s; (b) Strains at the interfaces of an 8ply laminate model C. DCZM Elements at Interfaces Based on the interface analysis carried out in the previous section, discrete cohesive zone method (DCZM) elements are added at the interfaces of the laminate to model delamination. The DCZM elements adopt a 1D traction law capable of simulating crack formation and propagation, i.e. delamination. The element features the ability to predict delamination initiation based on a traction law that captures the cohesive strength and the fracture toughness in each fracture mode (mode I, mode II and modeiii in the current model). The DCZM elements used in this paper have been successfully employed in other studies involving crack propagation as presented in. 25 A triangular tractionseparation law is used here. The inputs to the law are cohesive strengths in modei and modeii (σ c and τ c ), and fracture toughness in modei and modeii (G IC and G IIC ). The critical G IC and G IIC values are determined from the standard double cantilever beam (DCB) and edge notch flexure (ENF) tests, respectively (refer to 33 and 34 ). The modei cohesive strength is backed out from a DCB finite element virtual test, using experimentally determined modei fracture toughness as the input, and by varying the value of σ c until the loaddeflection response matches the one determined experimentally. The modeii cohesive strength is determined through a single lap joint test of 15
12 The experimentally determined fracture properties for the laminate are given in Table 5. Table 5. Fracture properties of interfaces in the laminate G IC G IIC σ c τ c 0.67 ± 0.07 N/mm 1.67 ± 0.08 N/mm 15 ± 2.5 MPa 28 ± 2 MPa It should be noted here that the fracture properties determined are between 0 degree layers in a laminate. Each interlaminar interface between laminae of different orientation could have different fracture properties, especially in modeii. But, here, the fracture properties between all the interfaces in the laminate are assumed to be the same. D. Effects of Stacking on Compressive Strength and Failure Mode: Comparison of Type A and Type B Laminates In order to study the effect of stacking sequence on the compressive strength and failure mode in Type A and Type B laminates, the upscaled homogenized model described above is implemented with interface elements (DCZM) added along the critical interfaces determined a priori from the 2D generalized plane strain analysis. Keeping the fracture toughnesses fixed at 0.67 N/mm and 1.67 N/mm in modei and modeii, the cohesive strengths are varied, and the corresponding global stressstrain responses are determined. A comparative investigation of Type A and Type B laminates is carried out in this section. The objective is to investigate the influence of stacking sequence on the compressive strength and failure mode in laminates. Therefore, the compressive response of the two different models was studied. The smallest model that represents the Type B 48 layer laminate is a 16 ply laminate with zero layers distributed through the thickness with a stacking sequence of [( 45/ + 45/90/0) 2 ]s. Type A 16ply laminate is constructed by scaling the thickness of the individual layers in Type A 8ply laminate. Compressive Strength (MPa) Experiment Type A Type B Mode II Cohesive Strength (MPa) (a) Compressive Strength (MPa) Type A Type B Experiment Imperfection Angle (degree) (b) Figure 12. (a) Variation of compressive strength of Type A and Type B laminates with varying modeii cohesive strength of the interfaces; (b) Imperfection sensitivity of Type A and Type B laminate models A slight imperfection is imparted to the model to account for fiber misalignment. Previous work 36 has shown that initial misalignment angles of 0.5 to 2 degrees of the zero laminae bound the distribution of fiber misalignment that is typical of carbon fiber reinforced prepreg aerospace laminates. The imperfection imparted here is closer to experimentally observed behavior, i.e., only the center zero layers are seeded with 12 of 15
13 an imperfection of θ = δ/l. This is because, during the manufacturing process, the pressure and temperature applied on the top of the laminate causes noticeable undulations in the 0 fibers, as opposed to offaxis layers. The initial state in the compression analysis is stress free. The compressive strengths are determined for the two laminates corresponding to modeii cohesive strengths in the range of MPa with an imperfection angle of 1 degree. The compressive strengths are plotted against modeii cohesive strengths in Fig. 12(a). Here, we observe that the compressive strengths of both the laminates increase with increasing modeii cohesive strengths. Further, the compressive strength of Type B laminate increases faster as compared to that of Type A laminate with an increase in modeii cohesive strength. This indicates that, due to distributed 0 degree layers in the Type B laminate, the kink band failure in these laminates is influenced more by the interface fracture properties as compared to the Type A laminate. Having said that, the distributed nature of the 0 layers in Type B laminates also makes the loading on the model more uniform as compared to Type A laminate, where the offaxis layers are subjected to higher stresses compared to the 0 layers. This leads to a nearly 10 % increase in the compressive strength in Type B laminates. Next, the influence of the imperfection angle on the compressive strength is studied. For a fixed value of modeii cohesive strength, the imperfection angle is varied from 1 degree to 1.5 degrees, which is within the range of imperfection angles measured in aerospace grade laminates. As expected, the compressive strength reduces with an increase in the imperfection angle. The sensitivity of compressive strength to changes in imperfection angle was similar in both Type A and Type B laminates as seen in Fig. 12(b). The deformation shapes of the two laminate models with the same material and fracture input properties are shown in Fig. 13(a), Fig. 13(b) and Fig. 13(c) corresponding to the initial linear stage, at peak load and in the postpeak regime of the stressstrain response respectively. (a) (b) (c) Figure 13. Deformation shapes of Type A and Type B laminates (a) in the initial linear regime, (b) at the peak load and (c) in the postpeak regime of the global stressstrain response It is noticed that, in both the laminates, delamination is accompanied by kink band formation. But, the kink band in the Type B laminate is restricted to a smaller zone compared to the Type A laminate. This implies that, even though the compressive strength is influenced by interface fracture properties in both the laminates, the growth or extent of delamination in Type B laminates is less compared to Type A laminates. 13 of 15
14 This observation is consistent with experimental observations, where it is noted that Type A laminates fail in a catastrophic manner, whereas Type B laminates, after kink banding and delamination, remain intact postexperiment (as shown in Fig. 1(b) and Fig. 1(d), respectively). This suggests that Type B laminates are favored over Type A laminates for structural applications. Indeed, standard laminate design practices limit the number of adjacent plies having the same angle. IV. Conclusions Computational models to predict the compressive strength were constructed based on failure mechanisms observed in experiments. The model facilitates delamination to occur along those interfaces that are prone to delamination by adding cohesive (DCZM) interface elements along the selected interfaces. These interfaces were determined apriori from the knowledge of the laminate stacking sequence and the geometry of the layers. The interfaces determined as the delamination prone interfaces match well with the experimentally observed delaminating interfaces. The properties of the DCZM elements were based on the interlaminar fracture properties that were determined experimentally. The predicted compressive strengths, when compared against the set of experimental results, were found to agree well, both in terms of the maximum load and the failure modes. The mode of failure is determined by the number and the orientation of the lamina in a laminate, the material shear nonlinearity (dictated by the matrix properties) and the interlaminar fracture properties. The methodology outlined in this paper can be used to quickly assess the compressive strength of laminates, within engineering limits, with a knowledge of the fundamental material properties as inputs. Thus, this method can be used very early in the design cycle of fiber reinforced laminated composite structures to establish design margins for strength allowables. That is, the compressive strength of the laminates with different combinations of layups, layer thicknesses and material properties can be investigated virtually. Further, only a handful of different types of laminates need to be manufactured and tested to decide on the final laminate to be used. This could result in a significant reduction of manufacturing and testing related costs. References 1 Schultheisz, C. R. and Waas, A. M., Compressive failure of composites.1. Testing and micromechanical theories, Progress in Aerospace Sciences, Vol. 32, No. 1, 1996, pp Waas, A. M. and Schultheisz, C. R., Compressive failure of composites.2. Experimental studies, Progress in Aerospace Sciences, Vol. 32, No. 1, 1996, pp Budiansky, B. and Fleck, N. A., Compressive failure of fiber composites, Journal of the Mechanics and Physics of Solids, Vol. 41, No. 1, 1993, pp Schapery, R. A., Prediction of compressive strength and kink bands in composites using a work potential, International Journal of Solids and Structures, Vol. 32, No. 67, 1995, pp Sun, C. T. and Jun, A. W., Compressive strength of unidirectional fiber composites with matrix nonlinearity, Composites Science and Technology, Vol. 52, No. 4, 1994, pp Kyriakides, S., Arseculeratne, R., Perry, E. J., and Liechti, K. M., On the compressive failure of fiberreinforced composites, International Journal of Solids and Structures, Vol. 32, No. 67, 1995, pp Lee, S. H. and Waas, A. M., Compressive response and failure of fiber reinforced unidirectional composites, International Journal of Fracture, Vol. 100, 1999, pp Vogler, T. J., Hsu, S. Y., and Kyriakides, S., On the initiation and growth of kink bands in fiber composites. Part II: analysis, International Journal of Solids and Structures, Vol. 38, 2001, pp Yerramalli, C. S. and Waas, A. M., A failure criterion for fiber reinforced polymer composites under combined compressiontorsion loading, International Journal of Solids and Structures, Vol. 40, No. 5, 2003, pp Yerramalli, C. S. and Waas, A. M., The effect of fiber diameter on the compressive strength of composites  A 3D finite element based study, Computer Modeling in Engineering and Sciences, Vol. 6, No. 1, 2004, pp Basu, S., Waas, A. M., and Ambur, D. R., Compressive failure of fiber composites under multiaxial loading, Journal of the Mechanics and Physics of Solids, Vol. 54, No. 3, 2006, pp Pimenta, S., Gutkin, R., Pinho, S. T., and Robinson, P., A micromechanical model for kinkband formation: Part I Experimental study and numerical modelling, Composites Science and Technology, Vol. 69, 2009, pp Pimenta, S., Gutkin, R., Pinho, S. T., and Robinson, P., A micromechanical model for kinkband formation: Part II Analytical modelling, Composites Science and Technology, Vol. 69, 2009, pp Feld, N., Allix, O., and Baranger, E., Micromechanical prediction of UD laminates behavior under combined compression up to failure: influence of matrix degradation, Journal of Composite Materials, Vol. 45, No. 22, 2011, pp Lee, S. H., Yerramalli, C. S., and Waas, A. M., Compressive splitting response of glassfiber reinforced unidirectional composites, Composites Science and Technology, Vol. 60, 2000, pp Waas, A. M., Babcock Jr., C. D., and Knauss, W. G., An experimental study of compression failure of fibrous laminated 14 of 15
15 composites in the presence of stress gradients, International Journal of Solids and Structures, Vol. 26, No. 910, 1990, pp Ahn, J. H. and Waas, A. M., A micromechanicsbased finite element model for compressive failure of notched uniply composite laminates under remote biaxial loads, Journal of Engineering Materials and Technology  Transactions of the ASME, Vol. 121, No. 3, 1999, pp Ahn, J. H. and Waas, A. M., Prediction of compressive failure in laminated composites at room and elevated temperature, AIAA Journal, Vol. 40, No. 2, 2002, pp Berbinau, P., Soutis, C., and Guz, I. A., Compressive failure of 0 0 unidirectional carbonfibrereinforced plastic (CFRP) laminates by fibre microbuckling, Composites Science and Technology, Vol. 59, 1999, pp Wisnom, M. R., The Effect of Fibre Waviness on the Relationship between Compressive and Flexural Strengths of Unidirectional Composites, Journal of Composite Materials, Vol. 28, Naik, N. K. and Kumar, R. S., Compressive strength of unidirectional composites: evaluation and comparison of prediction models, Composite Structures, Vol. 46, No. 3, 1999, pp Xu, Y. L. and Reifsnider, K. L., Micromechanical Modeling of Composite Compressive Strength, Journal of Composite Materials, Vol. 27, 1993, pp Yerramalli, C. S. and Waas, A. M., A nondimensional number to classify composite compressive failure, Journal of Applied Mechanics  Transactions of the ASME, Vol. 71, No. 3, 2004, pp Prabhakar, P. and Waas, A., Upscaling from a micromechanics model to capture laminate compressive strength due to kink banding instability, Computational Materials Science, Vol. 67, No. 0, 2013, pp Gustafson, P. and Waas, A., The influence of adhesive constitutive parameters in cohesive zone finite element models of adhesively bonded joints, International Journal of Solids and Structures, Vol. 46, No. 10, 2009, pp ARAMIS, ARAMIS Software Documentation, GOM Optical Measuring Teqhniques, Beghini, A., Bazant, Z. P., Waas, A. M., and Basu, S., Postcritical imperfection sensitivity of sandwich or homogenized orthotropic columns soft in shear and in transverse deformation, International Journal of Solids and Structures, Vol. 43, No , 2006, pp Pipes, R. B. and Pagano, N. J., Interlaminar Stresses in Composite Laminates Under Uniform Axial Extension, Journal of Composite Materials, Vol. 4, Pagano, N. and Pipes, R., The Influence of Stacking Sequence on Laminate Strength, Journal of Composite Materials, Vol. 5, No. 1, 1971, pp Pagano, N. and Pipes, R., Some observations on the interlaminar strength of composite laminates, International Journal of Mechanical Sciences, Vol. 15, No. 8, 1973, pp Martin, E., Leguillon, D., and Carrere, N., A twofold strength and toughness criterion for the onset of freeedge shear delamination in angleply laminates, International Journal of Solids and Structures, Vol. 47, No. 9, 2012, pp Pipes, R. B. and Daniel, I. M., Moiré Analysis of the Interlaminar Shear Edge Effect in Laminated Composites, Journal of Composite Materials, Vol. 5, ASTM(D5528), Standard Test Method for Mode I Interlaminar Fracture Toughness of Unidirectional FiberReinforced Polymer Matrix Composites, Davidson, B. D. and Sun, X., Geometry and Data Reduction Recommendations for a Standardized End Notched Flexure Test for Unidirectional Composites, Journal of ASTM International, Vol. 3, ASTM(D3165), Standard Test Method for Strength Properties of Adhesives in Shear by Tension Loading of SingleLap Joint Laminated Assemblies, Yurgartis, S. W., Measurement of small angle fiber misalignments in continuous fiber composites, Composites Science and Technology, Vol. 30, 1987, pp of 15
A Unified Model for Predicting the Open Hole Tensile and Compressive Strengths of Composite Laminates for Aerospace Applications
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationCompressive splitting failure of composites using modified shear lag theory
International Journal of Fracture 115: 27 40, 2002. 2002 Kluwer Academic Publishers. Printed in the Netherlands. Compressive splitting failure of composites using modified shear lag theory CHANDRA S. YERRAMALLI
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationREPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS
More informationPrediction of Compressive Strength of Fibrous Composites Using Two Different Approaches
Jordan Journal of Civil Engineering, Volume 8, No. 2, 214 Prediction of Compressive Strength of Fibrous Composites Using Two Different Approaches Yousef S. Al Rjoub 1) * and Karim S. Numayr 2) 1) Civil
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More informationModule 4: Behaviour of a LaminaeII. Learning Unit 1: M1. M4.1 Mechanics of Composites. M4.1.1 Introduction to Mechanics of Composites
Module 4: Behaviour of a LaminaeII Learning Unit 1: M1 M4.1 Mechanics of Composites M4.1.1 Introduction to Mechanics of Composites The relation between ply uniaxial strengths and constituent properties
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationFLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationIMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS OBTAINED WITH LMS SAMTECH SAMCEF
V ECCOMAS Thematic Conference on the Mechanical Response of Composites COMPOSITES 015 S.R. Hallett and J.J.C. Remmers (Editors) IMPACT ON LAMINATED COMPOSITE PLATES: COMPARISON OF TEST AND SIMULATION RESULTS
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationApplication of fracture mechanicsbased methodologies for failure predictions in composite structures
Application of fracture mechanicsbased methodologies for failure predictions in composite structures Zoltan Mikulik a, B. Gangadhara Prusty a, Rodney S. Thomson b, Donald W. Kelly a,* a School of Mechanical
More informationFinite ElementBased Failure Models for Carbon/Epoxy Tape Composites
Finite ElementBased Failure Models for Carbon/Epoxy Tape Composites A Master Thesis Presented to The Academic Faculty by Guillaume Seon In Partial Fulfillment of the Requirements for the Degree Master
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More informationFINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND
FINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND COMPARISON WITH EXPERIMENTAL IMPACT TESTS USING NONDESTRUCTIVE VIBROTHERMOGRAPHY EVALUATION A
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More information*MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials
14 th International LSDYNA Users Conference Session: Constitutive Modeling *MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials Jesper Karlsson 1, Mikael Schill 1, Johan Tryding
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationDESIGN OF LAMINATES FOR INPLANE LOADING
DESIGN OF LAMINATES FOR INPLANOADING G. VERCHERY ISMANS 44 avenue F.A. Bartholdi, 72000 Le Mans, France Georges.Verchery@m4x.org SUMMARY This work relates to the design of laminated structures primarily
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationAnálisis Computacional del Comportamiento de Falla de Hormigón Reforzado con Fibras Metálicas
San Miguel de Tucuman, Argentina September 14 th, 2011 Seminary on Análisis Computacional del Comportamiento de Falla de Hormigón Reforzado con Fibras Metálicas Antonio Caggiano 1, Guillermo Etse 2, Enzo
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More informationNUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION
NUMERICAL MODELLING OF COMPOSITE PIN JOINTS AND EXPERIMENTAL VALIDATION Fabrice PIERRON*, François CERISIER*, and Michel GRÉDIAC** * SMS/ Département Mécanique et Matériaux, École Nationale Supérieure
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationVIRTUAL TESTING OF ADVANCED POLYMER COMPOSITE MATERIALS. Ana Andreia Pinheiro Durão Branco. Master s Thesis Advisor: Prof. Dr. Pedro Ponces Camanho
VIRTUAL TESTING OF ADVANCED POLYMER COMPOSITE MATERIALS Ana Andreia Pinheiro Durão Branco Master s Thesis Advisor: Prof. Dr. Pedro Ponces Camanho Mestrado Integrado em Engenharia Mecânica July 17, 2015
More informationModeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress
Modeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress Authors Marco ANGHILERI * LuigiM L CASTELLETTI * Andrea MILANESE * and Andrea SEMBOLONI * Affiliation * Politecnico
More informationFREE EDGE DELAMINATION ONSET CRITERION
FREE EGE ELAMINATION ONSET CRITERION G. MARION now, 2, formerl 3, R. HARRY 2, and F. LECUYER MEYSYS, 29 rue J. Rostand, 9873 ORSAY CEEX, FRANCE 2 Laboratoire de Génie Mécanique, IUT Bordeaux I, 3345 TALENCE
More informationMechanical Design in Optical Engineering
OPTI Buckling Buckling and Stability: As we learned in the previous lectures, structures may fail in a variety of ways, depending on the materials, load and support conditions. We had two primary concerns:
More informationProgram: Recent Trends
The SNL/MSU/DOE Fatigue Program: Recent Trends John Mandell Montana State University 2012 SNL Blade Workshop May 30  June 1, 2012 Outline Overview of MSU Fatigue Program on Wind Blade Materials: Testing
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationInitiation de fissure dans les milieux fragiles  Prise en compte des contraintes résiduelles
Initiation de fissure dans les milieux fragiles  Prise en compte des contraintes résiduelles D. Leguillon Institut Jean le Rond d Alembert CNRS/UPMC Paris, France Parvizi, Garrett and Bailey experiments
More informationSTRAIN ASSESSMENT USFOS
1 STRAIN ASSESSMENT IN USFOS 2 CONTENTS: 1 Introduction...3 2 Revised strain calculation model...3 3 Strain predictions for various characteristic cases...4 3.1 Beam with concentrated load at mid span...
More informationFracture Behavior. Section
Section 6 Fracture Behavior In January 1943 the oneday old Liberty Ship, SS Schenectady, had just completed successful sea trials and returned to harbor in calm cool weather when... "Without warning and
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationDelamination in fractured laminated glass
Delamination in fractured laminated glass Caroline BUTCHART*, Mauro OVEREND a * Department of Engineering, University of Cambridge Trumpington Street, Cambridge, CB2 1PZ, UK cvb25@cam.ac.uk a Department
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationThis is a publisherdeposited version published in: Eprints ID: 4094
This is a publisherdeposited version published in: http://oatao.univtoulouse.fr/ Eprints ID: 4094 To cite this document: WEISS Ambrosius, TRABELSI Walid, MICHEL Laurent, BARRAU JeanJacques, MAHDI Stéphane.
More informationTESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationBACKGROUNDS. Two Models of Deformable Body. Distinct Element Method (DEM)
BACKGROUNDS Two Models of Deformable Body continuum rigidbody spring deformation expressed in terms of field variables assembly of rigidbodies connected by spring Distinct Element Method (DEM) simple
More information1.050 Content overview Engineering Mechanics I Content overview. Selection of boundary conditions: Euler buckling.
.050 Content overview.050 Engineering Mechanics I Lecture 34 How things fail and how to avoid it Additional notes energy approach I. Dimensional analysis. On monsters, mice and mushrooms Lectures 3. Similarity
More informationDetermination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors
Sensors 2012, 12, 1602416036; doi:10.3390/s121216024 Article OPEN ACCESS sensors ISSN 14248220 www.mdpi.com/journal/sensors Determination of the Shear Buckling Load of a Large Polymer Composite ISection
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationNumerical Characterization of Concrete Heterogeneity
Vol. Materials 5, No. Research, 3, 2002Vol. 5, No. 3, Statistical 309314, 2002. Characterization of the Concrete Numerical Modeling of Size Effect In Heterogeneity 2002 309 Numerical Characterization
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More information